Journal of Sol-Gel Science and Technology 32, 259–262, 2004 c
2004 Kluwer Academic Publishers. Manufactured in The United States.
Reduction of Eu3+
in Al-Codoped Silica Glasses Fabricated
by the Sol-Gel Technique and CO2
B. WILHELM∗, V. ROMANO AND H.P. WEBER
Institute of Applied Physics, University of Bern, Sidlerstrasse 5, 3012 Bern, Switzerland
Abstract. The spectroscopic properties of europium in aluminium codoped silica glasses produced by the sol-gel technique have been studied with respect to the dopant concentrations and the thermal processing applied to the samples. After thermal annealing at temperatures up to 950◦C the bright red fluorescence around 613 nm characteristic for the trivalent europium ions (Eu3+) has been observed. The lifetime was measured to be 0.1–2.4 ms depending on dopant concentrations and thermal treatment. Subsequent CO2-laser processing in air (short time
remelting) gave rise to a bright blue fluorescence consisting of two broad bands, lying around 450 and 490 nm, with their peak position depending on the ratio between the aluminium and europium concentrations. The fluorescence lifetimes were found to be shorter than 1µs. This blue fluorescence is attributed to the divalent europium ion (Eu2+), leading to the conclusion that the CO2-laser processing of europium doped alumina-silica glasses resulted in the
reduction of the trivalent to the divalent europium ion. Laser processing could therefore be a valid alternative to conventional thermal annealing for the generation of Eu2+in alumina-silica glasses.
Keywords: sol-gel, trivalent europium, divalent europium, alumina-silica glasses, CO2-laser
Rare earth ions or lanthanides in a glassy or crystalline host matrix are well known fluorescing materials and have therefore a wide range of applications from active materials for solid-state lasers and amplifiers to electro-optic devices and sensors. Europium is of particular interest for novel applications as trivalent ion with its luminescence in the orange-red as well as in its divalent configuration with a broad luminescence band from UV to blue-green [1, 2].
Trivalent europium is mainly used for remote high temperature sensing applications [3, 4], while crystals or ceramics doped with divalent europium ions find ap-plications as blue emitting phosphors for plasma dis-play panels and x-ray storage [5, 6]. Both forms of eu-ropium have been investigated in the past [e.g. 1, 2, 7] and even the transition from the trivalent to the
diva-∗Present address: School of Chemical and Physical Sciences,
Victo-ria University of Wellington, PO Box 600, Wellington, New Zealand. E-mail: firstname.lastname@example.org
lent ion at elevated temperatures and under a hydro-gen atmosphere has been reported [8, 9], but to our knowledge this reduction has not yet been observed during laser induced short time melting under ambient conditions.
We investigated the spectroscopic properties, such as fluorescence spectra and lifetime, of europium and, in some cases, aluminium doped sol-gel derived silica with respect to the thermal treatment applied to the samples and their dopant concentrations. In this paper we report the reduction of Eu3+ to Eu2+ in alumina-silica glasses during thermal processing with a CO2
Laser processing could therefore offer a fast alter-native to high temperature annealing under hydrogen atmosphere having the additional benefit of low sample contamination.
Glasses or glass-like silica samples were produced from a solution of tetraethoxysilane (TEOS) and
260 Wilhelm, Romano and Weber
additives by the sol-gel method, which is described in detail elsewhere . Dotation of the samples was achieved by adding europium nitrate hexahy-drate (Eu(NO3)3·6H2O) to this solution. Precursor
so-lutions with europium ion concentrations relative to silica atoms from 0.1 to 10% were prepared. By as-suming a final density of the samples equal to that of quartz glass, the europium concentration lies in the range of 2.2· 1019 to 2.2· 1021 cm−3. Aluminium
codoped samples were produced by adding an equal amount (0.1 to 10 at%) of aluminium nitrate nonahy-drate (Al(NO3)3·9H2O) or ten times more aluminium
(10% for a 1% europium doped sample) to the initial so-lution. The relative uncertainty of all concentrations is calculated to be approximately 10%. In the following, the samples are identified by their initial europium and, where applicable, aluminium concentration in atomic percent relative to Si.
Gelling of the solution and evaporation of solvents occurred at room temperature within several weeks, leading to monolithic samples of a size of several mm3.
Drying at moderate temperatures up to 250◦C lead to a further densification of the samples and evaporation of solvents.
The resulting samples were first examined without further thermal treatment. Subsequently the samples were annealed for several hours around 500 and 950◦C in a conventional oven or laser processed (melted) us-ing a CO2-laser. All thermal treatment was carried out
under ambient air.
The fluorescence spectra of the red emitting samples were measured with a fluorimeter, while the spectra of the blue emitting samples were recorded with an Ocean Optics USB Spectrometer using a continuously emit-ting UV lamp (peak wavelength 370 nm) for excitation. The fluorescence lifetimes were measured using a flashlamp (pulse length ∼10 µs, peak wavelength 370 nm) for excitation and a photomultiplier with a monochromator and a suitable interference filter for detection of the emission.
After drying at temperatures up to 250◦C the eu-ropium and eueu-ropium-aluminium doped silica sam-ples revealed the bright red fluorescence characteristic for the trivalent europium ion (Eu3+). Figure 1 shows the fluorescence spectrum recorded for a 10 at% eu-ropium doped silica sample. A series of sharp lines with FWHM∼10 nm, the main line lying at 613 nm,
Figure 1. Fluorescence spectrum of 10 at% Eu3+ doped sol-gel
was observed. Annealing at higher temperatures of 500 or 950◦C resulted in an unchanged fluorescence spec-trum.
The fluorescence lifetimes measured for the main emission line at 613 nm ranged from 0.13–2.40 ms, depending on the thermal treatment applied to the sam-ples and their europium and, where applicable, alu-minium concentration. The fluorescence lifetimes of silica samples doped with 1 at% europium are pre-sented in Table 1. It was found that the fluorescence lifetimes of europium in the aluminium modified silica host material are slightly shorter than the ones in the
Table 1. Fluorescence lifetimes (at 613 nm) for 1 at% europium doped silica samples depending on the aluminium concentration and the annealing temperature.
Al-concentration Annealing Fluorescence (at%) temperature (◦C) lifetime (ms)
0 250 0.17 0 500 0.43 0 950 2.40 0 CO2-laser –a 1 250 0.13 1 500 0.29 1 950 1.01 1 CO2-laser –b 10 250 0.13 10 500 0.33 10 950 1.54 10 CO2-laser –b aNo fluorescence observed. bBlue fluorescence observed.
Reduction of Eu3+to Eu2+in Al-Codoped Silica Glasses Fabricated 261
Figure 2. Fluorescence spectra of Eu2+in aluminium codoped sil-ica after CO2-laser processing and for different aluminium
corresponding pure silica and that the lifetimes gener-ally increased with increasing annealing temperature.
CO2-laser processing in air of the samples
contain-ing europium as well as aluminium gave rise to a bright blue fluorescence which is attributed to the di-valent europium ion (Eu2+) and comprises two broad bands (FWHM ∼100 nm) spaced by about 40 nm. It was found that their peak wavelengths depend on the sample composition. For samples doped with an equal amount of europium and aluminium (Al:Eu= 1) the peaks lie at 457± 4 and 497 ± 3 nm, the latter being the stronger peak, while for samples contain-ing more aluminium than europium (Al:Eu= 10) the peaks are slightly shifted to shorter wavelengths ly-ing at 444± 3 and 487 ± 2 nm and the former being the stronger peak. Furthermore all samples showed a small red fluorescence around 613 nm arising from a fraction of trivalent europium ions still present in the samples. Figure 2 shows the fluorescence spectra for two samples having the same europium concentration but different aluminium concentrations. The fluores-cence lifetimes could not be exactly determined, but were found to be shorter than 1µs for all samples.
CO2-laser processing of the europium doped silica
samples without aluminium did not lead to any observ-able blue fluorescence.
A typical fluorescence spectrum of the europium and, where applicable, aluminium doped samples annealed
at temperatures up to 950◦C is shown in Fig. 1 and reveals a series of sharp lines with FWHM ∼10 nm which is characteristic for the transition from the first excited state to the ground state of the 4f-electron in trivalent europium. We identified four separate lines at 578, 594, 613 and 653 nm associated with the transi-tions from the5D
0 level to the 7F0,7F1,7F2 and7F3
level, respectively. These values are in good agreement with literature [1, 7] and we therefore conclude that the europium is incorporated in the silica samples an-nealed at temperatures up to 950◦C in its trivalent form disregarding a potential aluminium codotation.
The observation of an increase in fluorescence life-time of one order of magnitude with increased anneal-ing temperature, as shown in Table 1, is explained by a reduced probability of concurring non-radiative de-cays associated with high-energy phonons present in the sol-gel derived host material. We have shown ear-lier , that a significant reduction of these phonons associated with OH-groups originating from solvents or not fully polymerised host material occurs during annealing at elevated temperatures and that this leads to a considerably prolonged fluorescence lifetime.
Similar results were found for samples doped with 0.1 and 10 at% europium, respectively, and for alu-minium codoped samples, although the increase in life-time was less pronounced for the samples containing 10 at% europium, presumably due to concentration quenching.
After CO2-laser processing, the europium and
alu-minium codoped silica samples revealed a bright blue fluorescence, as shown in Fig. 2, with fluorescence life-times shorter than 1µs.
We conclude, that this blue fluorescence is attributed to divalent europium ions (Eu2+) present in the host ma-terial after laser processing, since high purity chemicals (>99%) have been used to synthesise the samples and no other rare earth ions were present during the sol-gel process and the laser treatment. Furthermore blue fluorescence from Eu2+ is not unusual given that the ion readily emits light in a wide range from near UV to green, depending on the surrounding host material . In amorphous host materials and glass ceramics two peak emissions have been observed [9, 12] and the lifetimes given in literature  correspond with our measured upper limit of 1µs. It is also known, that the reduction of Eu3+to Eu2+ occurs at elevated temperatures of about 1100◦C in hydrogen atmosphere and can be reversed by applying an oxygen atmosphere [8, 9].
262 Wilhelm, Romano and Weber
The fluorescence spectra of all investigated samples doped with europium and aluminium were compara-ble after CO2-laser processing, all having two lines
but with slightly different peak wavelengths and in-tensity ratio of the two peaks. The evidence points in the direction of these differences being a function of the aluminium and europium concentrations. At low aluminium to europium ratios (Al:Eu = 1) the emis-sion at longer wavelength (494 nm) is stronger, while at higher ratios (Al:Eu = 10) the spectrum is shifted to shorter wavelengths and dominated by the line at 442 nm. Since the ground state for divalent europium consists of a single level (8S
7/2), we presume, that the
surrounding host material affects the position of the excited 5d1-level. The evidence suggests that two dif-ferent sites for the incorporation of the Eu2+ ion are present in the laser processed materials, even though they are amorphous, but further experiments will be carried out to corroborate this assumption.
Furthermore we discovered that during CO2-laser
processing in air the reduction of Eu3+to Eu2+is not complete. A small fraction of the ions remains in the trivalent state and their weak red fluorescence is still found in the fluorescence spectra. Further experiments are planned to clarify the conditions under which in-complete reduction occurs.
Our results show that CO2-laser processing under
ambient conditions allows to produce divalent eu-ropium in alumina-silica glasses and could therefore be a fast alternative to high temperature annealing in a hydrogen atmosphere, having the additional benefit of low sample contamination.
We investigated the spectroscopic properties of eu-ropium in aluminium codoped sol-gel derived silica in view of the dopant concentrations and thermal treat-ment. We found that CO2-laser processing of the
sam-ples gave rise to a bright blue fluorescence that consists of two broad lines with lifetimes shorter than 1 µs, and is attributed to divalent europium ions present in
the host material. The two emission lines are prob-ably associated with two different sites occupied by the europium ions in the host material and their peak wavelengths are related to the aluminium and europium concentration. We therefore conclude that a reduction of Eu3+to Eu2+occurs in aluminium doped silica dur-ing the CO2-laser treatment in air. Laser processing
turned out to be a fast and low contamination alter-native to high temperature annealing under hydrogen atmosphere.
This work was financed by the Swiss National Science Foundation (project 21-61517.00).
1. C.R. Kurkjian, P.K. Gallagher, W.R. Sinclair, and E.A. Sigety, Phys. Chem. Glasses 4, 239 (1963).
2. P. Dorenbos, J. Lumin. 104, 239 (2003).
3. M.R. Cates, S.W. Allison, G.J. Pogatshnik, and A.R. Bugos, Proc. SPIE 1375, 55 (1989).
4. B. Wilhelm, V. Romano, and H.P. Weber, in Proceedings of
TEMPMEKO 2001—8th International Symposium on Tempera-ture and Thermal Measurements in Industry and Science (VDE
Verlag GmbH, Berlin, 2002), p. 1131.
5. K. Yokota, S.X. Zhang, K. Kimura, and A. Sakamoto, J. Lumin.
92, 223 (2001).
6. A. Edgar, G.V.M. Williams, P.K.D. Sagar, M. Secu, S. Schweizer, J.M. Spaeth, X. Hu, P.J. Newman, and D.R. MacFarlane, J. Non-Cryst. Solids 326/327, 489 (2003). 7. H. Song, et al., J. Appl. Phys. 91, 2959 (2002). 8. Z. Gu, J. Non-Cryst. Solids 52, 337 (1982).
9. S.A. Studenikin and M. Cocivera, Thin Solid Films 394, 264 (2001).
10. C.J. Brinker and G.W. Scherer, Sol-Gel Science: The Physics and
Chemistry of Sol-Gel Processing (Academic Press, San Diego,
1990), ch. 3.
11. B. Wilhelm, V. Romano, and H.P. Weber, J. Non-Cryst. Solids
328, 192 (2003).
12. A. Edgar, S. Schweizer, S. Assmann, J.M. Spaeth, P.J. Newman, and D.R. MacFarlane, J. Non-Cryst. Solids 284, 237 (2001).
13. M. Secu, S. Schweizer, J.M. Spaeth, A. Edgar, G.V.M. Williams, and U. Rieser, J. Phys.: Condens. Matter 15, 1097 (2003).